Performance of Recycled HMA Mixes
Summit on Increasing RAP Usage
Randy West, DirectorNational Center for Asphalt Technology
Laboratory Research State Reports National Reports NCAT Test Track Summary
RAP in HMA is one of the most researched topics in the field of pavement materials.
Most of that research is based on laboratory testing.
That is a good place to start, but relating lab test results to field performance is like a preseason football poll.
Washington State WA-RD-98.1, 1986 Title: Hot Mix Recycling Evaluation in
Washington Authors: Peters, et al. Scope: 16 projects, RAP contents from
8 to 79% (half 70%), projects ranged from 1.5 to 10 years old
Washington State Findings:
WSDOT's initial two projectsare still performing very well.
The early data indicates equally promising results for the 14 other projects.
Because of the impressive pavement performance exhibited by the recycled pavements, benefits such as conservation of natural resources, and its cost advantage hot-mix recycling has become an attractive addition to the WSDOT paving program.
Louisiana LTRC Report No. 216, April 1995 Title: Evaluation of Recycled Projects for
Performance Author: Skip Paul Scope: 10 projects, RAP content: 20 to 50%,
data covered a six to nine years, evaluated pavement condition ratings, serviceability, structural analysis, and mix and binder properties
Findings pavements containing RAP performed
similarly to conventional mixtures for a period of six to nine years of service life
pavements with RAP exhibited slightly more distress with respect to longitudinal cracking
the substitution of up to 15 % [RAP in wearing courses] can provide acceptable performing pavements as long as the 12,000 poise viscosity limitation is maintained.
Report No.: FHWA-CTRD-647-4-87-1 Title: Performance Evaluation of Hot Mixed
Recycled Pavement Route 4, Burlington Authors: Ganung and Larsen Scope: conventional and 30% RAP,
performance compared at 6 years of service
Findings: No rutting was detected Roughness was low Extracted asphalt viscosities were higher for
recycled versus control, possibly explaining for the greater cracking on the recycled
This condition was reversed on the overlaid sections
Georgia TRR 1507, 1995 Title: Performance of Recycled Hot-Mix Asphalt
Mixtures in Georgia Authors: Kandhal, et al. Scope: Detailed comparison of 5 pairs of
recycled versus control projects, followed by comparison of a larger set of control and recycled HMA projects. RAP contents range from 10 to 25%
Findings: For the 5 paired comparisons, there was no
rutting, raveling, or fatigue cracking in either the recycled or conventional sections.
Comparison of recycled vs. conventional mixes on 15 projects indicated the RAP mixes performed equal to or better than the virgin mixes.
Title: Hot Mix Recycling in Massachusetts Scope: Rehabilitation project on I-295, 35% RAP
in binder layer, OGFC surface. The new binder in the RAP mix was adjusted to a softer grade.
Findings The pavement showed no distress after 11 years The RAP pavement performed better than the original
California Title: Comparative Analysis of Long-Term
Field Performance of Recycled Asphalt in California Environmental Zones, TRB 2008
Authors: Zaghloul and Holland Scope: 60 RAP sections (up to 15% RAP)
in 3 climatic zones in CA, evaluations at 5 to 9 years of service, rated by Structural Service Life, Distress Service Life, and Roughness Service Life
California Findings: Performance of RAP pavements
differs for the three climatic zones North Coast climatic zone Excellent to good
performance of pavements with RAP Mountain climatic zone structural
performance was marginal, but distress performance was poor
Desert climatic zone Structural performance was good but distress performance was poor
Granite Construction Title: Recycled Hot Mix Asphalt Performance in
Various Climatic Regions Authors: Robinette and Epps Scope and Approach:
Evaluated 114 conventional and recycled projects (10-35% RAP) on low-volume roads in 3 climatic regions: Low Desert, High Desert, & Coastal
Pavement ages from 1 to 10 years Visual condition surveys Predicted service lives
Robinette and Epps
Findings: Analyses of visual pavement condition
surveys indicate that recycled HMA pavements have a longer expected life for two of the three cases [climatic regions]
FHWA-SA-95-060, 1996 Pavement Recycling Executive Summary
and Report Author: Sullivan Scope: Review of HMA Recycling
Practices and Performance in 17 states
FHWA-SA-95-060 Conclusions Long-term pavement performance (17 years) show
that recycled HMA that is designed and controlled during production will perform comparably to conventional HMA and can improve material properties of the existing pavement layer.
Similar to poor performing conventional HMA, poor recycled HMA performance can be related to poor mix design procedures or use of control and acceptance procedures that do little to ensure the quality of the recycled HMA.
Recycled HMA, which is designed and produced in a quality assurance program that verifies mix design assumptions to reasonable limits, can be expected to perform comparably to conventional HMA.
LTPP Study: RAP vs. Virgin Mixtures
Report: FHWA-RD-98, June 1998 Title: Performance Trends of Rehabilitated
Asphalt Concrete Pavements in the LTPP Experiments: Initial Observations
Researcher: Brent Rauhut Engineering Scope: SPS-5 and GPS-6 sections
factors: overlay thickness, milling, and RAP RAP sections contained 30% RAP from project
LTPP Study: RAP vs. Virgin MixturesPlus 2 Canadian Provinces
LTPP Study: Findings Rutting - ...there is no important difference in
resistance of rutting between virgin and recycled mixes.
Fatigue - The recycled mixtures have a higher percentage of sections with fatigue cracking compared to the virgin mixtures, but exhibit on the average smaller areas of cracking.
Thermal Cracking - In general, it is believed that mixtures with RAP are stiffer (or more brittle) and more susceptible to thermal fracture. The initial performance observations seem to contradict the debatable hypothesis.
Texas Follow Up on SPS-5
In TRB Circular E-C078, October 2005 Title: Lessons Learned from the Long-
Term Pavement Performance Program and Several Recycled Sections in Texas
Authors: Chen and Daleiden Scope: Five TXDOT SPS-5 projects with
30% RAP and virgin HMA sections and one nearby Hot-In-Place recycled pavement
Texas Follow Up on SPS-5 Findings:
After more than 10 years of service, the RAP sections perform as well as the virgin asphalt concrete (AC) sections.
All SPS-5 sections are able to resist reflective cracking when a mixture of 30% RAP and a softer binder is used, the result is a high penetration number (30 to 45), with a flexible mixture able to resist cracking.
In contrast, cracks came through the HIP recycled sections in just a few weeks for US-175 and US-84. Low penetration numbers in the range of 20 to 21 were found.
Experience with RAPon the NCAT Test Track
Use of RAP in the First Two Cycles of the NCAT Test Track
2000 FDOT S6 & S7 15% RAP PG 67-22 20 million ESALs, 5 years
Use of RAP in the First Two Cycles of the NCAT Test Track
2006 TNDOT S6, MSDOT S2 15% RAP PG 76-22 9 million ESALs No rutting No raveling No cracking
NCAT TEST TRACKRAP Experiment
RAP Test Sections
NCAT Test Track RAP Sections
1. virgin control mix with PG 67-222. 20% RAP with PG 67-22 virgin binder3. 20% RAP with PG 76-22 virgin binder4. 45% RAP with PG 52-28 virgin binder5. 45% RAP with PG 67-22 virgin binder6. 45% RAP with PG 76-22 virgin binder7. 45% RAP with PG 76-22 + Sasobit
Determine the appropriate grade of virgin binder needed for High RAP mixes.
Assess constructability of high RAP mixes Mix design issues Plant issues Paving and compaction
Accelerated Traffic Performance Compare rutting over time Compare cracking and durability
-3/16 RAP+3/4 RAP
3/4 x 3/16 RAPIn back
Recycled Mix Production
Coarse (3/4 3/16) RAP Bin Fine (-3/16) RAP Bin
Mix QC Summaries
Mix Virgin Control 20% RAP 45% RAP
NMAS 12.5 12.5 12.5
Pb 5.8% 5.6 5.8% 4.9 5.1%
Va 2.9% 1.9 2.1% 1.7 3.6%
VMA 15.9% 14.2 14.5% 12.5 13.9%
95% 92 94% 94 96%
Test Section Construction
E7-45%RAP PG76-22 +Sasobit
Rutting Performance @ 9.0M ESALs
Virgin + PG 67-22
20% RAP+ PG 67-22
20% RAP+ PG 76-22
45% RAP+ PG 52-28
45% RAP+ PG 67-22
45% RAP+ PG 76-22
Click here to load reader